Figure 3. Curves of optical transmittance versus wavelength for different grades of carbon nanotubes and ITO show relatively flat transmittance for nanotubes across the visible spectral region. All transmittance values refer to the transparent conductor layer only, with substrate effect removed.
Measures of optical transmittance versus wavelength for carbon nanotube films show reduced optical transmittance with decreasing sheet resistance (see figure 3). A useful attribute of the material is demonstrated in the flatness of the curves across the visible spectrum. In contrast, ITO shows stronger absorbance at shorter wavelengths in the visible range (hence, its characteristic yellow color). Carbon nanotube films exhibit neutral color, a big advantage for display applications.
The nanotubes also exhibit other useful properties such as electrical conductivities as high as 100 Ω-1/cm-1, plus high strength, thermal conductivity, and flexibility. To test their flexibility and response to strain, we made carbon nanotube test samples by spray coating heat-stabilized, 125-µm-thick polyester (PET) film with purified carbon nanotube dispersion. We then dipped the film in a melamine/acrylic binder solution, air dried, and cured it. The nanotube/binder stack was about 75-nm thick, with sheet resistance of about 650 Ω/square and visible-light transmittance of 90%. We subjected the samples to up to 18% strain at a 0.1 mm/min strain rate in uni-axial tension at 25°C. For comparison, we tested commercially available ITO films with sheet resistance of about 250 Ω/square and PET films 125 µm thick. The resultant plot of change in resistance (ΔR/R0) versus strain (ΔL/L0) shows the stability and robustness of carbon nanotubes compared to ITO.
In cycle testing, carbon nanotube films showed no signs of cracking until about 27,000 cycles, with failure observed at about 32,000 cycles. To put the carbon nanotube performance into perspective, 25,000 cycles is roughly equivalent to seven years of use for a roll-out flexible display device flexed every day, 10 times per day. In comparison, ITO films developed cracks that led to catastrophic failure (open circuit) at about 6000 cycles.
Based on scanning electron microscope images of the failed nanotube films, we attribute the ultimate failure to agglomerates in the film (point defects that act as stress concentrators). The melamine/acrylic binder is also more brittle than other binder resins we have used. We plan to do additional work to improve the quality of carbon nanotube dispersion and use more flexible/ductile binder resins. Circuitry and Displays
Conductive carbon nanotube structures can produce transparent circuits on display substrates, offering a method for fabricating flexible displays. We have tested three methods for fabricating transparent circuits and electrodes from carbon nanotubes. Each uses a two-step approach in which we form the carbon nanotube layer and then add a polymeric binder topcoat. This two-step approach yields improved optoelectronic properties for the carbon nanotube layer and enables some simple circuit fabrication methodologies.
In the first method, we feed the PET substrate into a standard laser jet printer to print a negative image of the desired circuit in styrene carbon-block ink (standard printer ink). The nanotubes are extremely durable; they deform but they spring back. If a hole is punched in them, they reform. The carbon nanotube layer is deposited by a wet coating method. We use spray application with ultrasonic or airbrush methods, but other techniques like dipping or roll coating are compatible. Next we dip the carbon-nanotube-coated film in organic solvent (toluene) for 3 s to remove the negative image, leaving behind the patterned carbon nanotube layer. A polymeric topcoat applied over the top protects the carbon nanotube circuit.
In the second method, we deposit the carbon nanotube film over the entire substrate surface and pattern it with a polymer binder material like amorphous fluoropolymer or polyester. We can pattern the binder with screen printing, ink jet printing, or other methods. Rinsing the substrate with a water/surfactant solution removes the unprotected carbon nanotube regions.
In the third method, we print the carbon nanotube pattern directly on the substrate. Several different methods to print the carbon nanotube layer are currently being studied, including ink jet printing, focused-beam spray, screen printing, and gravure roll printing. This third approach is very attractive because it results in the least waste and has the simplest manufacturing flow.
There is no inherent technological barrier limiting the use of carbon nanotube films for applications in which ITO is currently used. At this point in the development of the technology, however, specifically with regard to the resistance verses transmittance properties, there is further work to do to meet the needs of some display applications.
The material has been evaluated with very encouraging results in various electrophoretic or reflective display technologies for which higher resistance (1 K Ω/square to 100 K Ω/square) is acceptable and for which the very high transmittance (better than 95% at 550 nm) of the material at these resistance values is especially important. Dozens of full-size reflective displays incorporating carbon nanotube circuitry are currently operating in various laboratories and long-term testing for brightness and durability is underway. Initial results are very promising. Brightness is improved by approximately 8 to 10% over ITO in most of these displays, with less change as the display ages.
In addition, these durable coatings are potentially important for touch screens; qualification tests are underway. These display technologies are expected to be early adopters. Other applications include LCD television circuitry.
OLED displays are also quite demanding from an RS/%T performance standpoint, since the conductors must have sheet resistance below 50 Ω/square and transparency better than 90%T. An application of this technology to OLED displays will thus take several years longer than that of the other display types. This is also true for application to plasma television electrodes.
Much progress has been made with this technology but its full potential has only begun to be exploited. In the next year, research and development will continue to push the performance of the coatings toward meeting the most demanding applications, while focusing on commercial production and leveraging the existing level of technology. oe
1. B. Lewis, D. Paine, MRS Bulletin. Aug 2000 p. 22 (2000).
2. S. Ijima et al., Science 306, p. 1362 (2004).
The authors would like to thank Professor G. Crawford and J. Vedrine from Brown University for their help with mechanical reliability testing. We gratefully acknowledge the following people for their guidance and support: P. Black, RDEC, Redstone, Army; K. Johnson, AFRL, WPAFB; J. Connell, NASA Langley.
Paul Glatkowski, Phillip Wallis, Michael Trottier
Paul Glatkowski is vice president of engineering, Phillip Wallis is technical director, and Michael Trottier is senior engineer at Eikos Inc., Franklin, MA.